Replica-Exchange Molecular Dynamics Simulations of Cellulose Solvated in Water and in the Ionic Liquid 1‑Butyl-3Methylimidazolium Chloride Barmak Mostoﬁan,†,‡ Xiaolin Cheng,†,§ and Jeremy C. Smith*,†,§ †
UT/ORNL Center for Molecular Biophysics, Oak Ridge National Laboratory, Oak Ridge, Tennessee 37830, United States Graduate School of Genome Science and Technology, The University of Tennessee, Knoxville, Tennessee 37996, United States § Department of Biochemistry, Cellular & Molecular Biology, The University of Tennessee, Knoxville, Tennessee 37996, United States ‡
S Supporting Information *
ABSTRACT: Ionic liquids have become a popular solvent for cellulose pretreatment in bioreﬁneries due to their eﬃciency in dissolution and their reusability. Understanding the interactions between cations, anions, and cellulose is key to the development of better solvents and the improvement of pretreatment conditions. While previous studies described the interactions between ionic liquids and cellulose ﬁbers, shedding light on the initial stages of the cellulose dissolution process, we study the end state of that process by exploring the structure and dynamics of a single cellulose decamer solvated in 1-butyl-3-methyl-imidazolium chloride (BmimCl) and in water using replica-exchange molecular dynamics. In both solvents, global structural features of the cellulose chain are similar. However, analyses of local structural properties show that cellulose explores greater conformational variability in the ionic liquid than in water. For instance, in BmimCl the cellulose intramolecular hydrogen bond O3H′···O5 is disrupted more often resulting in greater ﬂexibility of the solute. Our results indicate that the cellulose chain is more dynamic in BmimCl than in water, which may play a role in the favorable dissolution of cellulose in the ionic liquid. Calculation of the conﬁgurational entropy of the cellulose decamer conﬁrms its higher conformational ﬂexibility in BmimCl than in water at elevated temperatures.
1. INTRODUCTION Ionic liquids (ILs) are low melting point salts that are usually ﬂuid below 100 °C. They often consist of an organic cation and a smaller anion. Because of their low volatility and reusability, ILs have been suggested to be of potential use in several industrial processes that involve chemical separation or synthesis.1−6 One important ﬁeld of application for ILs is the nonderivatized dissolution of lignocellulosic biomass before enzymatic hydrolysis.7−11 In particular, the decomposition of cellulose, a glucose polymer that occurs in a ﬁbrillar structure in plant cell walls, into smaller fermentable sugars has been shown to be more eﬃcient after substrate pretreatment with imidazolium-based ILs.12−17 Improved eﬃciency in biomass pretreatment is essential to the development of a sustainable biofuel industry based on renewable resources.18−20 To this end, considerable research eﬀorts have been focused on the search for ILs that facilitate cellulose dissolution,21−24 as well as on understanding the molecular mechanisms that govern the dissolution process.25−31 Molecular dynamics (MD) simulations are useful in the analysis of interactions at atomic detail. Several MD studies have examined the eﬀects of solvation of cellulose in water32−34 or the free energy of single-chain detachment from microﬁbrils in aqueous solution.35,36 Simulations of crystalline cellulose ﬁbers in ILs such as 1-butyl-3-methylimidazolium chloride © 2014 American Chemical Society
(BmimCl) or 1-ethyl-3-methylimidazolium acetate (EmimAc), which contain cations with an aromatic head and an aliphatic tail group, have revealed conformational changes of cellulose induced by the ionic solvent.37,38 Recent studies have conﬁrmed the hypothesis that anions, which usually have greater hydrogen bond basicity and thus make stronger hydrogen bonds with cellulose than water oxygens,9 facilitate cellulose dissolution by breaking its intramolecular hydrogen bonds.39 It has also been suggested that the less polar cation participates in the dissolution process, for example, through stacking and intercalation.40−43 This ﬁnding seems plausible given the fact that cellulose is an amphiphilic molecule with exposed hydroxyl groups and hydrophobic pyranose rings. Hence, for eﬃcient cellulose dissolution, both polar and nonpolar solvent components may be required44,45 as provided by the most commonly used ILs. The dissolution of cellulose by ILs involves the transition from the ﬁber state to the fully dissolved state of individual chains.46 All-atom simulation of this entire process is not currently feasible due to the large system size (generally > 100 000 atoms) and the concomitant timescale limitation to the Received: March 24, 2014 Revised: August 25, 2014 Published: September 2, 2014 11037
dx.doi.org/10.1021/jp502889c | J. Phys. Chem. B 2014, 118, 11037−11049
The Journal of Physical Chemistry B
sub-μs regime. Therefore, many previous studies have been focused on the simulation of a cellulose ﬁber solvated in water or in ILs, which sheds light on the initial stages of the dissolution process. Here, we study a single fully dissolved cellulose chain, which provides a description of the ﬁnal state of dissolution. The comparative analysis of the thermodynamic and dynamic behavior of a cellulose chain fully solvated in water and in an IL can reveal diﬀerences in the eﬀects of these two solvents, leading to a better understanding of the diﬀerential dissolution process and its driving forces. Previously, short simulations ( 14 Å. (c) Fraction of extended (Rg > 14 Å, solid lines) and compact (Rg < 14 Å, dashed lines) structures for cellulose in BmimCl (black) and in water (red).
increasing temperature. The polysaccharide does not collapse to a compact structure with increasing temperature but rather gradually reduces its stiﬀness and thus samples more conformations of smaller overall size at higher T. This behavior is qualitatively diﬀerent from that in proteins that denature and expand upon increasing temperature and fold into a compact native state structure at lower, physiological temperatures. Negligible changes in the solvent-accessible surface area and in the solvent-excluded volume of cellulose (Supporting Information, Figure S4) both conﬁrm that a sharp transition from an extended to a compact conformation does not occur. The fact that the decrease of Rg or d as a function of the temperature is comparable in both solvents means that this temperature-dependent conformational change is not driven by speciﬁc interactions of the solute with water molecules or with BmimCl ions. However, in BmimCl both proﬁles show greater variation at any temperature as indicated by the larger error
∑ (ri(O4) − rmean(O4))2 i
where rmean(O4) is the average position of the oxygen atom and Ng = 9 is the number of glycosidic bonds. The sampled cellulose conformations range from elongated decamer structures to collapsed conﬁgurations (see Supporting Information, Figure S3). Temperature proﬁles based on Rg (Figure 2a) or on the cellulose end-to-end distance d (Supporting Information, Figure S3) both indicate that in both solvents the overall size of the decamer reduces with 11039
dx.doi.org/10.1021/jp502889c | J. Phys. Chem. B 2014, 118, 11037−11049
The Journal of Physical Chemistry B
Figure 3. (a) Probability distributions of the cellulose hydroxymethyl angle ω (displayed on the far right) in BmimCl (left) and in water (right) for the four temperatures T = 375, 400, 425, and 450 K. The two preferred conformations around ω = −60° and ω = 60° are referred to as GG and GT, respectively. Colors correspond to the given temperatures (see far right). (b) Temperature proﬁles of occupancies for cellulose intramolecular hydrogen bonds O3H′···O6, O2H···O6′, O6H′···O2, and O3H′···O5 (displayed on the far right) between any two neighboring glucose units in BmimCl (left) and in water (right). Only the O3H′···O5 hydrogen bond is formed to a signiﬁcant degree. Colors correspond to the given bonds (see far right).
bars, suggesting higher ﬂexibility of cellulose in the IL than in water. On the basis of the value of Rg, any given cellulose decamer structure can be broadly classiﬁed as compact (Rg < 14 Å) or extended (Rg > 14 Å). According to this classiﬁcation, in both solvents at any temperature the majority of all sampled cellulose structures is extended (Figure 2b). Interestingly, while ∼90% of cellulose structures are extended at the lowest simulation temperature, only ∼55% are extended at the highest temperatures (Figure 2c). This shows that the REMD approach broadly explores conformational space, sampling both compact and extended cellulose conformations at any temperature. The cellulose decamer behaves like a semirigid rod polymer at lower temperatures, which is characteristic at length scales below a polymer’s persistence length, LP.67 The values of LP of cellulose in aqueous solution at room temperature reported in the literature are between ∼100 and ∼160 Å, signiﬁcantly longer than the contour length of the decamer studied here.68−70 By extrapolation, in the present REMD simulations LP for the decamer is indeed estimated to be >10 glucose units at T < 400 K but decreases to 5 glucose units (∼26 Å) at T = 500 K in both solvents (Supporting Information, Figure S5). This explains why the cellulose decamer is mainly extended at lower temperatures and collapsed at higher temperatures in this study. The polymer structure of cellulose in the simulations is characterized and discussed in more detail in the Supporting Information. Except for the greater ﬂexibility of the solute in BmimCl, the present results on overall structural parameters such as the radius of gyration and the persistence length do not reveal a signiﬁcant diﬀerence between the two solvents. However, in addition to these parameters, we investigated the rotamer
conformations of the hydroxymethyl groups and the glycosidic bonds as well as the ability to form intramolecular hydrogen bonds or to maintain the six-membered ring of its glucose units in the favorable chair conformation (pyranose ring puckering). The hydroxymethyl group of a glucose unit can adopt stable staggered rotamers, referred to as GG, GT, and TG, corresponding to the trans and gauche conformations of the O5−C5−C6−O6 and C4−C5−C6−O6 torsions. We deﬁne the angle ω as the former torsion. The distributions of ω at distinct temperatures for simulations in BmimCl and in water are given in Figure 3a. The TG conformation is populated at 14 Å) cellulose chains (data not shown). In the Iα and Iβ forms of crystalline cellulose, intramolecular hydrogen bonds exist between O3H′···O5, O3H′···O6, O2H··· O6′, and O6H′···O2 of neighboring monomers (where the prime labels the residue toward the reducing end).71 In this study, we consider a hydrogen bond formed when the donor− acceptor distance is 80% can be attributed to basin O,